synthetic polymer scaffolds for soft tissue synthetic polymer scaffolds for soft tissue engineering
Post on 23-Jan-2020
Embed Size (px)
PHYSIOLOGICAL RESEARCH • ISSN 0862-8408 (print) • ISSN 1802-9973 (online) 2018 Institute of Physiology of the Czech Academy of Sciences, Prague, Czech Republic Fax +420 241 062 164, e-mail: firstname.lastname@example.org, www.biomed.cas.cz/physiolres
Physiol. Res. 67 (Suppl. 2): S335-S348, 2018
Synthetic Polymer Scaffolds for Soft Tissue Engineering
1Department of Biological Models, Institute of Macromolecular Chemistry of the Czech Academy of Sciences, Prague, Czech Republic
Received May 31, 2018 Accepted July 11, 2018
Summary Tissue engineering (TE) and regenerative medicine are progressively developed areas due to many novel tissue replacements and implementation strategies. Increasing knowledge involving the fabrication of biomaterials with advanced physicochemical and biological characteristics, successful isolation and preparation of stem cells, incorporation of growth and differentiation factors, and biomimetic environments gives us a unique opportunity to develop various types of scaffolds for TE. The current strategies for soft tissue reconstitution or regeneration highlight the importance of novel regenerative therapies in cases of significant soft tissue loss and in cases of congenital defects, disease, trauma and ageing. Various types of biomaterials and scaffolds have been tested for soft tissue regeneration. The synthetic types of materials have gained great attention due to high versatility, tunability and easy functionalization for better biocompatibility. This article reviews the current materials that are usually the most used for the fabrication of scaffolds for soft TE; in addition, the types of scaffolds together with examples of their applications for the regenerative purposes of soft tissue, as well as their major physicochemical characteristics regarding the increased applicability of these materials in medicine, are reviewed.
Key words Synthetic 3D scaffolds • Soft tissue regeneration • Tissue engineering
Corresponding author O. Janouskova, Department of Biological Models, Institute of Macromolecular Chemistry of the Czech Academy of Sciences, Heyrovského nám. 2, 162 06 Prague 6, Czech Republic. E-mail: email@example.com
In the 1990s, Langer and Vacanti first defined the term “tissue engineering” (TE) (Langer and Vacanti 1993). TE combines the fields of cell biology, biomaterial engineering and medicine to produce new functional tissues. The three main components that are required for the reconstitution or regeneration of damaged or diseased tissue are as follows: i) harvested cells from donor tissue; ii) biomaterial scaffolds, which support cell attachment, proliferation and/or differentiation, as well as possess sufficient physicochemical properties; and iii) chemical signals, such as cytokines and growth factors. The scaffolds play a major role in TE strategies. Three-dimensional (3D) scaffolds have been usually used to provide a structurally stable environment for tissue regeneration. A scaffold serves as an artificial extracellular matrix (ECM). A native ECM is a 3D network whose composition and structure interact with the cells and provide structural support, transfer mechanical forces and allow the transport of chemical signals.
Scaffold materials can be based on natural or synthetic polymers. They can be degradable or non-degradable, depending on the specific use. Natural polymers were among the first biodegradable scaffolds, which were clinically used for TE purposes (Dhandayuthapani et al. 2011), preferentially due to their better overall interaction with various cell types and lack of an immune response (Nair 2007). Synthetic polymers are largely studied and applied for TE. They were discovered to be cheaper and more easily functionalized than natural polymers, despite the potential for immune
S336 Janoušková Vol. 67 response or cytotoxicity depending on the used polymer materials and synthetic processes, which can include toxic substances. These types of polymers are highly useful in biomedical fields for their properties e.g. porosity, degradation time and mechanical characteristics. Desired properties can be tailored for specific applications. They can be produced under controlled conditions and in large uniform quantities. They exhibit predictable, reproducible, mechanical and physical properties such as strength, elastic modulus, and degradation rate. The synthetic polymer scaffolds are widely combined with natural polymers, naturally isolated proteins or peptides to improve, for example, hydrophobicity, cell attachment and biodegradability.
Materials for TE should have mechanical properties suitable for reconstructing or replacing damaged tissues. Moreover, the materials must be biocompatible, meaning that they are non-cytotoxic, do not cause excessive immune responses, must be capable of mimicking ECM, and provide an optimal support for cell adhesion and proliferation, facilitating cell-to-cell contact and cell migration. The materials should further be majorly bioabsorbable over the appropriate time frame, being necessary for replacement by growing tissue, and the materials must be adaptable to scaffold manufacturing techniques.
Soft TE has been developed as an advanced strategy to repair damage in soft tissue or diseased soft tissues in the case when the natural ability of the body to repair small or moderate sized tissue damage has failed, and the process of reparation remains the real problem. Soft tissue covers a variety of tissues, such as skin, tendon, muscle, cartilage, nerves, fascia, intervertebral disc or blood vessels. These tissues often have supporting or connecting functions of the body structures and organs. Frequently in everyday life, soft tissue damage caused by congenital defects, disease, trauma and ageing often leads to non-self-healable defects (Xu et al. 2014). Autologous implantation is the first method of treating the defects or disease. Unfortunately, it has been shown that autologous tissue can be easily absorbed, and only up to 60 % of soft tissue cells remain viable (Bauer-Kreisel et al. 2010). In this view, the TE has been used to develop new biological substitutes to overcome barriers of current clinical treatments for repairing and regenerating damaged or diseased of soft tissues and organs.
This review is focused on providing an overview of the synthetic biomaterials used for scaffold fabrication for soft tissue reparation, the classification of the most
prevalent type of scaffolds, their important physicochemical characterizations in regard to soft tissue engineering applications, and examples of experimental and clinical applications. Physicochemical characteristics of scaffolds
Scaffolds serve as an active instrument to provide guidance for the formation of new tissue. Through known physicochemical properties and biological functions of damaged tissue, the scaffolds should be fabricated. The required characteristics are as follows:
1) External geometry, which influences interconnectivity 2) Porosity and pore size 3) Mechanical properties 4) Degradation properties 5) Biocompatibility and susceptibility to hosting cells
Surface properties such as surface area, charge, and chemical modification External geometry
Scaffolds should mimic a natural ECM in damaged tissue in such a way as to provide structural support and tensile strength, offer an attachment site or cell surface receptors that later influence tissue formation, and finally initiate regeneration. The scaffolds are prepared from nano- to macro-scale structural geometry. In the geometry of scaffolds, the maintenance of highly interconnected porous fabrics of high surface density has to be addressed. This maintenance can favor the better infiltration of cells, growth and regenerative components of the scaffold. Porosity and pore size
Porosity is one of the major factors for the appropriate ingrowth of cells and vascularisation. Pore size, pore distribution, pore volume, pore interconnectivity, pore shape, and pore wall roughness have to be addressed during the design of the scaffold. These pore properties are crucial for the growth of new tissues and their reorganization, which includes building up the cellular network and interconnected pathways for nutrient transportation, cell signalling and proliferation. The optimum pore sizes for neovascularization were demonstrated experimentally and were 5 µm (Brauker et al. 1995), 5-15 µm for fibroblast ingrowth (Klawitter and Hulbert 1971), 20 µm for hepatocyte ingrowth (Yang et al. 2001), or 20-125 µm for regeneration of adult
2018 Soft Tissue Engineering S337
mammalian skin (Whang et al. 1999). It is also crucial to ensure the cells are approximately 200 µm from the blood supply to provide sufficient oxygen and nutrient transfer (Yang et al. 2001). In addition to appropriate porosity, the mechanical strength of the scaffolds has to be retained. Mechanical properties
The biostability of many scaffolds relies on factors such as strength, elasticity, and absorption at the material interface and given the chemical degradation of the material. These properties have to encourage the regeneration of the tissue. The biomaterial scaffold should also temporarily resist and conduct the loads and stresses that the new tissue can ultimately bear. It is important to evaluate rheological parameters, such as i) elastic modulus – measured strain in response to a given compressive stress along th